#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/51/24/1512402.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1512402
loop_
_publ_author_name
'Xing Meng'
'Hai-Ning Wang'
'Xin-Long Wang'
'Guang-Sheng Yang'
'Shuang Wang'
'Kui-Zhan Shao'
'Zhong-Min Su'
_publ_section_title
;
 Construction and property investigation of inorganic-organic hybrid
 materials based on metal-salens and Keggin polyoxometalates
;
_journal_name_full
;
Inorganica Chimica Acta
;
_journal_page_first              135
_journal_page_last               142
_journal_paper_doi               10.1016/j.ica.2012.04.011
_journal_volume                  390
_journal_year                    2012
_chemical_formula_moiety         'C64 H60 Cu6 N8 O50 Si W12'
_chemical_formula_sum            'C64 H60 Cu6 N8 O50 Si W12'
_chemical_formula_weight         4356.73
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 90.000(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            4
_cell_length_a                   14.939(5)
_cell_length_b                   23.406(5)
_cell_length_c                   34.243(5)
_cell_measurement_reflns_used    58870
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.31
_cell_measurement_theta_min      1.19
_cell_volume                     11973(5)
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97(Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.1242
_diffrn_reflns_av_sigmaI/netI    0.1042
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -41
_diffrn_reflns_number            58870
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.31
_diffrn_reflns_theta_min         1.19
_exptl_absorpt_coefficient_mu    12.599
_exptl_absorpt_correction_T_max  0.061
_exptl_absorpt_correction_T_min  0.055
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.417
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             7904
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.22
_platon_squeeze_details          ' ?'
_refine_diff_density_max         2.481
_refine_diff_density_min         -4.088
_refine_diff_density_rms         0.293
_refine_ls_extinction_coef       0.000015(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.960
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     614
_refine_ls_number_reflns         10859
_refine_ls_number_restraints     410
_refine_ls_restrained_S_all      1.051
_refine_ls_R_factor_all          0.1190
_refine_ls_R_factor_gt           0.0692
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1127P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1853
_refine_ls_wR_factor_ref         0.2084
_reflns_number_gt                5758
_reflns_number_total             10859
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ICA-2012-390-135-142-4.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      'Pbca '
_cod_database_code               1512402
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'-x-1/2, y-1/2, z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
C1 C -0.3553(15) 0.0045(11) 0.8135(8) 0.080(7) Uani 1 1 d .
C2 C -0.3401(15) -0.0040(11) 0.8513(7) 0.078(7) Uani 1 1 d U
H2 H -0.3047 0.0234 0.8635 0.093 Uiso 1 1 calc R
C3 C -0.371(2) -0.0490(16) 0.8756(11) 0.154(12) Uani 1 1 d U
H3 H -0.3610 -0.0509 0.9024 0.184 Uiso 1 1 calc R
C4 C -0.421(2) -0.0941(17) 0.8518(11) 0.154(12) Uani 1 1 d .
H4 H -0.4400 -0.1280 0.8634 0.184 Uiso 1 1 calc R
C5 C -0.4365(16) -0.0841(11) 0.8161(9) 0.094(9) Uani 1 1 d .
H5 H -0.4718 -0.1103 0.8027 0.113 Uiso 1 1 calc R
C6 C -0.4033(13) -0.0343(10) 0.7939(7) 0.061(6) Uani 1 1 d .
C7 C -0.4269(13) -0.0295(10) 0.7522(8) 0.076(7) Uani 1 1 d .
H7 H -0.4617 -0.0586 0.7417 0.091 Uiso 1 1 calc R
C8 C -0.4393(15) 0.0118(12) 0.6894(6) 0.087(9) Uani 1 1 d .
H8A H -0.4507 -0.0267 0.6800 0.105 Uiso 1 1 calc R
H8B H -0.4950 0.0330 0.6885 0.105 Uiso 1 1 calc R
C9 C -0.3755(17) 0.0382(12) 0.6659(7) 0.088(5) Uani 1 1 d .
H9A H -0.4050 0.0545 0.6432 0.106 Uiso 1 1 calc R
H9B H -0.3333 0.0097 0.6567 0.106 Uiso 1 1 calc R
C10 C -0.2935(17) 0.1295(12) 0.6703(7) 0.078(7) Uani 1 1 d .
H10 H -0.2997 0.1310 0.6433 0.093 Uiso 1 1 calc R
C11 C -0.2511(15) 0.1763(12) 0.6879(8) 0.079(8) Uani 1 1 d .
C12 C -0.2378(12) 0.1809(9) 0.7283(7) 0.057(6) Uani 1 1 d .
C13 C -0.1926(16) 0.2284(11) 0.7442(7) 0.091(9) Uani 1 1 d D
H13 H -0.1852 0.2320 0.7710 0.110 Uiso 1 1 calc R
C14 C -0.1582(15) 0.2711(12) 0.7181(8) 0.091(6) Uani 1 1 d .
H14 H -0.1256 0.3014 0.7283 0.109 Uiso 1 1 calc R
C15 C -0.1718(15) 0.2684(12) 0.6791(6) 0.091(6) Uani 1 1 d DU
H15 H -0.1503 0.2967 0.6625 0.109 Uiso 1 1 calc R
C16 C -0.2201(17) 0.2209(12) 0.6647(9) 0.098(8) Uani 1 1 d U
H16 H -0.2319 0.2194 0.6381 0.117 Uiso 1 1 calc R
C17 C -0.1447(15) 0.0029(12) 0.7281(7) 0.080(6) Uani 1 1 d U
C18 C -0.1891(14) -0.0479(11) 0.7470(9) 0.087(8) Uani 1 1 d .
H18 H -0.1960 -0.0493 0.7740 0.105 Uiso 1 1 calc R
C19 C -0.2200(15) -0.0932(11) 0.7235(12) 0.102(11) Uani 1 1 d .
H19 H -0.2412 -0.1256 0.7362 0.122 Uiso 1 1 calc R
C20 C -0.221(2) -0.0934(16) 0.6871(11) 0.113(11) Uani 1 1 d U
H20 H -0.2529 -0.1214 0.6738 0.136 Uiso 1 1 calc R
C21 C -0.1812(19) -0.0572(14) 0.6693(9) 0.102(9) Uani 1 1 d U
H21 H -0.1760 -0.0633 0.6425 0.123 Uiso 1 1 calc R
C22 C -0.1394(16) -0.0046(13) 0.6842(8) 0.089(6) Uani 1 1 d .
C23 C -0.0957(16) 0.0443(13) 0.6634(8) 0.089(6) Uani 1 1 d .
H23 H -0.0994 0.0430 0.6363 0.107 Uiso 1 1 calc R
C24 C -0.011(2) 0.1233(13) 0.6495(8) 0.111(8) Uani 1 1 d U
H24A H -0.0543 0.1470 0.6363 0.134 Uiso 1 1 calc R
H24B H 0.0198 0.1003 0.6300 0.134 Uiso 1 1 calc R
C25 C 0.0540(18) 0.1594(13) 0.6693(8) 0.095(6) Uani 1 1 d U
H25A H 0.1129 0.1420 0.6682 0.114 Uiso 1 1 calc R
H25B H 0.0571 0.1963 0.6566 0.114 Uiso 1 1 calc R
C26 C 0.0588(15) 0.2094(11) 0.7273(7) 0.070(7) Uani 1 1 d .
H26 H 0.0942 0.2348 0.7133 0.084 Uiso 1 1 calc R
C27 C 0.0434(12) 0.2210(9) 0.7681(6) 0.058(4) Uani 1 1 d U
C28 C 0.0766(13) 0.2713(11) 0.7826(7) 0.073(5) Uani 1 1 d U
H28 H 0.1035 0.2973 0.7657 0.088 Uiso 1 1 calc R
C29 C 0.0706(13) 0.2842(10) 0.8229(8) 0.073(5) Uani 1 1 d U
H29 H 0.0951 0.3180 0.8323 0.088 Uiso 1 1 calc R
C30 C 0.0283(15) 0.2466(9) 0.8484(7) 0.070(5) Uani 1 1 d U
H30 H 0.0221 0.2547 0.8749 0.084 Uiso 1 1 calc R
C31 C -0.0028(13) 0.1982(9) 0.8328(6) 0.057(4) Uani 1 1 d U
H31 H -0.0276 0.1717 0.8500 0.068 Uiso 1 1 calc R
C32 C -0.0020(13) 0.1832(9) 0.7933(6) 0.058(4) Uani 1 1 d U
N1 N -0.3248(14) 0.0849(11) 0.6871(5) 0.088(5) Uani 1 1 d .
N2 N -0.4048(11) 0.0099(8) 0.7297(5) 0.060(5) Uani 1 1 d .
N3 N -0.0551(14) 0.0866(9) 0.6769(6) 0.074(5) Uani 1 1 d U
N4 N 0.0271(13) 0.1665(8) 0.7095(6) 0.071(4) Uani 1 1 d U
O1 O 0.3207(12) 0.0166(9) 0.9439(5) 0.111(7) Uani 1 1 d .
O2 O -0.0411(16) 0.0475(11) 0.9683(7) 0.056(6) Uani 0.50 1 d PU
O1W O -0.2168(16) 0.1475(10) 0.8510(6) 0.1625(16) Uani 1 1 d DU
O3 O -0.0290(19) -0.0297(12) 0.9612(7) 0.0617(3) Uani 0.50 1 d PU
O3' O 0.0792(16) -0.0360(12) 0.9781(8) 0.058(6) Uani 0.50 1 d PU
O6 O 0.2272(13) -0.0558(8) 0.9952(5) 0.117(7) Uani 1 1 d .
O7 O 0.1636(12) 0.0767(8) 0.9386(5) 0.104(6) Uani 1 1 d U
O8 O 0.1625(13) -0.0365(8) 0.9233(5) 0.108(6) Uani 1 1 d U
O9 O 0.1130(15) -0.1266(8) 0.9622(6) 0.114(7) Uani 1 1 d U
O10 O -0.0499(11) -0.1168(8) 0.9325(5) 0.100(6) Uani 1 1 d .
O11 O 0.2251(11) 0.0517(8) 1.0085(5) 0.096(4) Uani 1 1 d U
O12 O 0.0022(13) -0.0252(7) 0.8959(6) 0.103(6) Uani 1 1 d U
O13 O 0.1168(13) 0.1391(8) 0.9997(5) 0.104(6) Uani 1 1 d U
O14 O -0.0458(12) 0.1466(10) 0.9692(6) 0.120(7) Uani 1 1 d U
O15 O -0.1178(12) 0.0498(9) 0.7507(4) 0.115(3) Uani 1 1 d DU
O16 O 0.0909(13) -0.1251(9) 0.8831(6) 0.118(7) Uani 1 1 d U
O17 O 0.2277(13) -0.1647(7) 1.0213(5) 0.101(6) Uani 1 1 d .
O18 O -0.0002(12) 0.0865(8) 0.9085(5) 0.103(6) Uani 1 1 d U
O19 O -0.1270(9) 0.0385(8) 0.8606(4) 0.080(5) Uani 1 1 d .
O20 O 0.2235(13) 0.1429(8) 1.0617(7) 0.124(7) Uani 1 1 d U
O21 O -0.1609(13) 0.0730(10) 0.9379(6) 0.125(7) Uani 1 1 d U
O22 O 0.0978(12) 0.1824(7) 0.9254(4) 0.083(5) Uani 1 1 d .
O23 O 0.0831(13) 0.0417(10) 0.9941(6) 0.0387(14) Uani 0.50 1 d PU
O24 O -0.0426(9) 0.1348(8) 0.7814(6) 0.112(3) Uani 1 1 d DU
O25 O -0.3169(12) 0.0498(9) 0.7972(6) 0.109(3) Uani 1 1 d U
O26 O -0.1580(11) -0.0328(8) 0.9220(5) 0.099(6) Uani 1 1 d .
O27 O -0.2593(12) 0.1398(9) 0.7534(6) 0.113(3) Uani 1 1 d U
Si1 Si 0.0000 0.0000 1.0000 0.0387(14) Uani 1 2 d SU
Cu1 Cu -0.32740(15) 0.07280(11) 0.74288(7) 0.0553(6) Uani 1 1 d U
Cu2 Cu -0.04642(17) 0.10747(11) 0.72884(7) 0.0583(7) Uani 1 1 d U
Cu3 Cu -0.1769(4) 0.0974(2) 0.80642(17) 0.1625(16) Uani 1 1 d DU
W1 W -0.08643(6) 0.02744(4) 0.90623(2) 0.0608(3) Uani 1 1 d .
W2 W 0.21816(6) 0.01134(5) 0.96127(3) 0.0700(3) Uani 1 1 d U
W3 W 0.06538(6) -0.08652(4) 0.92064(3) 0.0617(3) Uani 1 1 d U
W4 W 0.15498(7) 0.09504(4) 1.04213(3) 0.0674(3) Uani 1 1 d U
W5 W 0.06519(8) 0.12404(4) 0.94920(3) 0.0729(3) Uani 1 1 d U
W6 W 0.15400(7) -0.11173(5) 1.01434(3) 0.0747(3) Uani 1 1 d U
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O25 C1 C2 117(2) . .
O25 C1 C6 124(2) . .
C2 C1 C6 119(2) . .
C1 C2 C3 129(3) . .
C2 C3 C4 111(3) . .
C5 C4 C3 118(3) . .
C4 C5 C6 126(3) . .
C1 C6 C7 124(2) . .
C1 C6 C5 117(2) . .
C7 C6 C5 119(2) . .
N2 C7 C6 126(2) . .
C9 C8 N2 108.4(19) . .
C8 C9 N1 113(2) . .
N1 C10 C11 128(2) . .
C10 C11 C16 120(3) . .
C10 C11 C12 123(2) . .
C16 C11 C12 117(3) . .
O27 C12 C11 123(2) . .
O27 C12 C13 116(2) . .
C11 C12 C13 121(2) . .
C12 C13 C14 119(2) . .
C15 C14 C13 122(3) . .
C14 C15 C16 117(2) . .
C11 C16 C15 124(3) . .
O15 C17 C18 120(2) . .
O15 C17 C22 129(2) . .
C18 C17 C22 111(3) . .
C19 C18 C17 120(3) . .
C20 C19 C18 125(4) . .
C21 C20 C19 120(4) . .
C20 C21 C22 128(4) . .
C21 C22 C23 131(3) . .
C21 C22 C17 115(3) . .
C23 C22 C17 114(3) . .
N3 C23 C22 130(3) . .
N3 C24 C25 111(2) . .
N4 C25 C24 109(2) . .
N4 C26 C27 124(2) . .
C28 C27 C32 120(2) . .
C28 C27 C26 117(2) . .
C32 C27 C26 123(2) . .
C27 C28 C29 121(2) . .
C30 C29 C28 120(2) . .
C31 C30 C29 116(2) . .
C30 C31 C32 127(2) . .
O24 C32 C31 119.9(19) . .
O24 C32 C27 124(2) . .
C31 C32 C27 116(2) . .
C10 N1 C9 124(2) . .
C10 N1 Cu1 125(2) . .
C9 N1 Cu1 110.9(17) . .
C7 N2 C8 121(2) . .
C7 N2 Cu1 125.4(16) . .
C8 N2 Cu1 114.0(15) . .
C23 N3 C24 117(2) . .
C23 N3 Cu2 127(2) . .
C24 N3 Cu2 116.0(18) . .
C26 N4 C25 116(2) . .
C26 N4 Cu2 129.0(17) . .
C25 N4 Cu2 114.5(17) . .
Si1 O2 W1 125.3(14) . .
Si1 O2 W6 121.8(13) . 5_557
W1 O2 W6 98.9(9) . 5_557
Si1 O2 W5 114.6(12) . .
W1 O2 W5 95.4(9) . .
W6 O2 W5 93.7(9) 5_557 .
Si1 O3 O3' 59.5(13) . .
Si1 O3 O23 57.1(11) . 5_557
O3' O3 O23 97.3(17) . 5_557
Si1 O3 W3 125.5(15) . .
O3' O3 W3 66.0(12) . .
O23 O3 W3 133.7(16) 5_557 .
Si1 O3 W4 122.4(14) . 5_557
O3' O3 W4 133.5(17) . 5_557
O23 O3 W4 65.3(11) 5_557 5_557
W3 O3 W4 94.5(9) . 5_557
Si1 O3 W1 120.4(14) . .
O3' O3 W1 129.1(17) . .
O23 O3 W1 126.4(15) 5_557 .
W3 O3 W1 93.6(9) . .
W4 O3 W1 92.0(9) 5_557 .
Si1 O3' O3 55.3(11) . .
Si1 O3' W3 126.2(13) . .
O3 O3' W3 70.9(12) . .
Si1 O3' W2 119.6(14) . .
O3 O3' W2 133.1(17) . .
W3 O3' W2 96.2(9) . .
Si1 O3' W6 118.3(14) . .
O3 O3' W6 131.6(17) . .
W3 O3' W6 95.9(10) . .
W2 O3' W6 93.5(8) . .
W6 O6 W2 138.3(10) . .
W5 O7 W2 137.2(11) . .
W3 O8 W2 137.7(11) . .
W3 O9 W6 138.4(11) . .
W4 O10 W3 139.3(12) 5_557 .
W4 O11 W2 141.1(10) . .
W1 O12 W3 140.4(11) . .
W4 O13 W5 135.9(11) . .
W5 O14 W6 138.0(13) . 5_557
C17 O15 Cu2 120.5(14) . .
C17 O15 Cu3 134.6(15) . .
Cu2 O15 Cu3 101.1(8) . .
W1 O18 W5 135.4(11) . .
W1 O19 Cu3 154.2(10) . .
W6 O21 W1 138.1(13) 5_557 .
Si1 O23 O3 55.3(11) . 5_557
Si1 O23 W4 126.9(12) . .
O3 O23 W4 71.5(12) 5_557 .
Si1 O23 W2 121.9(12) . .
O3 O23 W2 138.1(14) 5_557 .
W4 O23 W2 95.8(7) . .
Si1 O23 W5 118.0(10) . .
O3 O23 W5 128.1(14) 5_557 .
W4 O23 W5 94.1(8) . .
W2 O23 W5 91.7(7) . .
C32 O24 Cu2 125.4(13) . .
C32 O24 Cu3 126.1(14) . .
Cu2 O24 Cu3 101.1(7) . .
C1 O25 Cu1 126.0(18) . .
C1 O25 Cu3 134.0(16) . .
Cu1 O25 Cu3 93.9(8) . .
W1 O26 W4 139.2(9) . 5_557
C12 O27 Cu1 127.2(18) . .
C12 O27 Cu3 131.4(15) . .
Cu1 O27 Cu3 94.4(9) . .
O3 Si1 O3 180.000(10) . 5_557
O3 Si1 O23 112.5(13) . .
O3 Si1 O23 67.5(13) 5_557 .
O3 Si1 O23 67.5(13) . 5_557
O3 Si1 O23 112.5(13) 5_557 5_557
O23 Si1 O23 180.0(13) . 5_557
O3 Si1 O3' 65.2(14) . .
O3 Si1 O3' 114.8(14) 5_557 .
O23 Si1 O3' 72.2(12) . .
O23 Si1 O3' 107.8(12) 5_557 .
O3 Si1 O3' 114.8(14) . 5_557
O3 Si1 O3' 65.2(14) 5_557 5_557
O23 Si1 O3' 107.8(12) . 5_557
O23 Si1 O3' 72.2(12) 5_557 5_557
O3' Si1 O3' 180.0(17) . 5_557
O3 Si1 O2 111.0(13) . 5_557
O3 Si1 O2 69.0(13) 5_557 5_557
O23 Si1 O2 101.8(12) . 5_557
O23 Si1 O2 78.2(12) 5_557 5_557
O3' Si1 O2 71.9(13) . 5_557
O3' Si1 O2 108.1(13) 5_557 5_557
O3 Si1 O2 69.0(13) . .
O3 Si1 O2 111.0(13) 5_557 .
O23 Si1 O2 78.2(12) . .
O23 Si1 O2 101.8(12) 5_557 .
O3' Si1 O2 108.1(13) . .
O3' Si1 O2 71.9(13) 5_557 .
O2 Si1 O2 180.0(13) 5_557 .
O27 Cu1 N2 174.3(8) . .
O27 Cu1 N1 93.1(10) . .
N2 Cu1 N1 83.9(9) . .
O27 Cu1 O25 90.3(9) . .
N2 Cu1 O25 93.5(8) . .
N1 Cu1 O25 170.4(9) . .
N3 Cu2 O15 98.8(8) . .
N3 Cu2 N4 84.0(9) . .
O15 Cu2 N4 177.1(8) . .
N3 Cu2 O24 175.2(8) . .
O15 Cu2 O24 83.3(6) . .
N4 Cu2 O24 93.9(8) . .
O1W Cu3 O24 108.1(9) . .
O1W Cu3 O15 171.8(10) . .
O24 Cu3 O15 64.3(7) . .
O1W Cu3 O25 96.4(9) . .
O24 Cu3 O25 150.8(7) . .
O15 Cu3 O25 90.0(7) . .
O1W Cu3 O27 100.3(9) . .
O24 Cu3 O27 90.5(7) . .
O15 Cu3 O27 77.2(7) . .
O25 Cu3 O27 69.2(7) . .
O1W Cu3 O19 81.0(9) . .
O24 Cu3 O19 103.2(6) . .
O15 Cu3 O19 103.5(7) . .
O25 Cu3 O19 96.0(6) . .
O27 Cu3 O19 165.2(6) . .
O19 W1 O12 100.5(8) . .
O19 W1 O26 100.3(8) . .
O12 W1 O26 87.8(8) . .
O19 W1 O18 99.8(8) . .
O12 W1 O18 90.4(8) . .
O26 W1 O18 159.8(8) . .
O19 W1 O21 103.5(9) . .
O12 W1 O21 155.9(9) . .
O26 W1 O21 85.5(9) . .
O18 W1 O21 88.0(8) . .
O19 W1 O2 159.0(9) . .
O12 W1 O2 95.9(9) . .
O26 W1 O2 93.2(9) . .
O18 W1 O2 67.0(9) . .
O21 W1 O2 61.5(9) . .
O19 W1 O3 155.7(9) . .
O12 W1 O3 62.2(8) . .
O26 W1 O3 64.2(8) . .
O18 W1 O3 97.3(9) . .
O21 W1 O3 94.2(9) . .
O2 W1 O3 45.2(9) . .
O1 W2 O11 102.9(9) . .
O1 W2 O7 101.0(9) . .
O11 W2 O7 88.3(7) . .
O1 W2 O8 101.7(9) . .
O11 W2 O8 155.2(8) . .
O7 W2 O8 90.5(8) . .
O1 W2 O6 102.1(9) . .
O11 W2 O6 83.6(8) . .
O7 W2 O6 156.7(9) . .
O8 W2 O6 87.9(7) . .
O1 W2 O23 157.2(9) . .
O11 W2 O23 59.8(7) . .
O7 W2 O23 66.1(8) . .
O8 W2 O23 97.3(8) . .
O6 W2 O23 91.0(9) . .
O1 W2 O3' 156.4(10) . .
O11 W2 O3' 94.1(8) . .
O7 W2 O3' 95.7(9) . .
O8 W2 O3' 61.4(8) . .
O6 W2 O3' 63.3(9) . .
O23 W2 O3' 46.3(8) . .
O16 W3 O9 103.8(10) . .
O16 W3 O8 101.8(10) . .
O9 W3 O8 89.0(8) . .
O16 W3 O10 100.1(10) . .
O9 W3 O10 89.7(9) . .
O8 W3 O10 157.7(9) . .
O16 W3 O12 100.5(10) . .
O9 W3 O12 155.6(9) . .
O8 W3 O12 86.2(8) . .
O10 W3 O12 85.9(7) . .
O16 W3 O3' 160.8(10) . .
O9 W3 O3' 64.4(10) . .
O8 W3 O3' 64.4(9) . .
O10 W3 O3' 95.1(9) . .
O12 W3 O3' 92.1(9) . .
O16 W3 O3 156.1(10) . .
O9 W3 O3 93.6(10) . .
O8 W3 O3 94.7(10) . .
O10 W3 O3 63.2(9) . .
O12 W3 O3 63.1(9) . .
O3' W3 O3 43.1(9) . .
O20 W4 O11 105.8(9) . .
O20 W4 O10 98.4(10) . 5_557
O11 W4 O10 155.8(8) . 5_557
O20 W4 O13 97.4(10) . .
O11 W4 O13 89.5(8) . .
O10 W4 O13 87.3(8) 5_557 .
O20 W4 O26 104.0(10) . 5_557
O11 W4 O26 88.2(8) . 5_557
O10 W4 O26 85.9(8) 5_557 5_557
O13 W4 O26 158.3(8) . 5_557
O20 W4 O23 158.8(10) . .
O11 W4 O23 61.9(7) . .
O10 W4 O23 95.0(8) 5_557 .
O13 W4 O23 66.8(8) . .
O26 W4 O23 93.2(8) 5_557 .
O20 W4 O3 157.4(10) . 5_557
O11 W4 O3 93.6(8) . 5_557
O10 W4 O3 62.7(9) 5_557 5_557
O13 W4 O3 94.3(9) . 5_557
O26 W4 O3 64.3(8) 5_557 5_557
O23 W4 O3 43.2(8) . 5_557
O22 W5 O14 101.9(9) . .
O22 W5 O7 99.2(9) . .
O14 W5 O7 158.8(9) . .
O22 W5 O18 99.8(8) . .
O14 W5 O18 86.8(8) . .
O7 W5 O18 89.3(8) . .
O22 W5 O13 99.9(8) . .
O14 W5 O13 88.6(8) . .
O7 W5 O13 88.1(8) . .
O18 W5 O13 160.3(8) . .
O22 W5 O2 155.4(8) . .
O14 W5 O2 62.6(9) . .
O7 W5 O2 97.3(9) . .
O18 W5 O2 62.3(8) . .
O13 W5 O2 98.7(8) . .
O22 W5 O23 155.5(8) . .
O14 W5 O23 95.1(9) . .
O7 W5 O23 64.9(8) . .
O18 W5 O23 98.7(8) . .
O13 W5 O23 62.7(8) . .
O2 W5 O23 49.1(7) . .
O17 W6 O6 100.8(9) . .
O17 W6 O21 101.3(10) . 5_557
O6 W6 O21 86.2(9) . 5_557
O17 W6 O14 101.5(10) . 5_557
O6 W6 O14 157.7(10) . 5_557
O21 W6 O14 89.7(9) 5_557 5_557
O17 W6 O9 102.1(9) . .
O6 W6 O9 89.2(8) . .
O21 W6 O9 156.6(10) 5_557 .
O14 W6 O9 85.8(9) 5_557 .
O17 W6 O2 156.1(9) . 5_557
O6 W6 O2 93.6(9) . 5_557
O21 W6 O2 60.4(9) 5_557 5_557
O14 W6 O2 65.5(9) 5_557 5_557
O9 W6 O2 97.1(9) . 5_557
O17 W6 O3' 155.9(9) . .
O6 W6 O3' 64.5(8) . .
O21 W6 O3' 96.8(10) 5_557 .
O14 W6 O3' 94.3(9) 5_557 .
O9 W6 O3' 60.8(9) . .
O2 W6 O3' 48.0(9) 5_557 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 O25 1.33(3) .
C1 C2 1.33(3) .
C1 C6 1.34(3) .
C2 C3 1.42(3) .
C3 C4 1.53(5) .
C4 C5 1.27(4) .
C5 C6 1.48(3) .
C6 C7 1.47(3) .
C7 N2 1.25(3) .
C8 C9 1.39(3) .
C8 N2 1.47(2) .
C9 N1 1.52(3) .
C10 N1 1.28(3) .
C10 C11 1.40(4) .
C11 C16 1.39(3) .
C11 C12 1.40(3) .
C12 O27 1.33(3) .
C12 C13 1.41(3) .
C13 C14 1.43(3) .
C14 C15 1.35(3) .
C15 C16 1.41(4) .
C17 O15 1.40(3) .
C17 C18 1.51(3) .
C17 C22 1.51(3) .
C18 C19 1.41(4) .
C19 C20 1.25(4) .
C20 C21 1.20(4) .
C21 C22 1.47(4) .
C22 C23 1.50(4) .
C23 N3 1.25(3) .
C24 N3 1.44(3) .
C24 C25 1.45(3) .
C25 N4 1.44(3) .
C26 N4 1.27(3) .
C26 C27 1.44(3) .
C27 C28 1.37(3) .
C27 C32 1.41(3) .
C28 C29 1.42(3) .
C29 C30 1.39(3) .
C30 C31 1.34(3) .
C31 C32 1.40(3) .
C32 O24 1.35(2) .
N1 Cu1 1.93(2) .
N2 Cu1 1.926(18) .
N3 Cu2 1.85(2) .
N4 Cu2 1.885(19) .
O1 W2 1.648(17) .
O2 Si1 1.67(3) .
O2 W1 2.28(3) .
O2 W6 2.34(3) 5_557
O2 W5 2.48(3) .
O1W Cu3 2.015(10) .
O3 Si1 1.56(3) .
O3 O3' 1.72(4) .
O3 O23 1.75(3) 5_557
O3 W3 2.39(3) .
O3 W4 2.43(3) 5_557
O3 W1 2.46(3) .
O3' Si1 1.64(3) .
O3' W3 2.31(3) .
O3' W2 2.42(2) .
O3' W6 2.43(3) .
O6 W6 1.829(18) .
O6 W2 1.958(16) .
O7 W5 1.876(18) .
O7 W2 1.899(18) .
O8 W3 1.867(17) .
O8 W2 1.908(19) .
O9 W3 1.847(17) .
O9 W6 1.92(2) .
O10 W4 1.866(17) 5_557
O10 W3 1.906(17) .
O11 W4 1.859(17) .
O11 W2 1.874(18) .
O12 W1 1.843(19) .
O12 W3 1.915(16) .
O13 W4 1.869(18) .
O13 W5 1.927(19) .
O14 W5 1.870(19) .
O14 W6 1.896(18) 5_557
O15 Cu2 1.88(2) .
O15 Cu3 2.380(10) .
O16 W3 1.617(19) .
O17 W6 1.675(16) .
O18 W1 1.892(17) .
O18 W5 1.915(17) .
O19 W1 1.696(14) .
O19 Cu3 2.428(16) .
O20 W4 1.658(19) .
O21 W6 1.87(2) 5_557
O21 W1 1.89(2) .
O22 W5 1.663(15) .
O23 Si1 1.59(2) .
O23 O3 1.75(3) 5_557
O23 W4 2.33(2) .
O23 W2 2.42(2) .
O23 W5 2.48(2) .
O24 Cu2 1.91(2) .
O24 Cu3 2.350(10) .
O25 Cu1 1.94(2) .
O25 Cu3 2.39(2) .
O26 W1 1.851(15) .
O26 W4 1.905(15) 5_557
O27 Cu1 1.90(2) .
O27 Cu3 2.41(2) .
Si1 O3 1.56(3) 5_557
Si1 O23 1.59(2) 5_557
Si1 O3' 1.64(3) 5_557
Si1 O2 1.67(3) 5_557
W4 O10 1.866(17) 5_557
W4 O26 1.905(15) 5_557
W4 O3 2.43(3) 5_557
W6 O21 1.87(2) 5_557
W6 O14 1.896(18) 5_557
W6 O2 2.34(3) 5_557
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O25 C1 C2 C3 -178(3) . .
C6 C1 C2 C3 -2(5) . .
C1 C2 C3 C4 5(5) . .
C2 C3 C4 C5 -6(5) . .
C3 C4 C5 C6 6(6) . .
O25 C1 C6 C7 -6(4) . .
C2 C1 C6 C7 178(2) . .
O25 C1 C6 C5 176(2) . .
C2 C1 C6 C5 0(4) . .
C4 C5 C6 C1 -2(5) . .
C4 C5 C6 C7 179(3) . .
C1 C6 C7 N2 1(4) . .
C5 C6 C7 N2 179(2) . .
N2 C8 C9 N1 -34(3) . .
N1 C10 C11 C16 179(2) . .
N1 C10 C11 C12 -1(4) . .
C10 C11 C12 O27 4(3) . .
C16 C11 C12 O27 -176(2) . .
C10 C11 C12 C13 178(2) . .
C16 C11 C12 C13 -2(3) . .
O27 C12 C13 C14 173(2) . .
C11 C12 C13 C14 -2(3) . .
C12 C13 C14 C15 3(4) . .
C13 C14 C15 C16 -1(4) . .
C10 C11 C16 C15 -176(2) . .
C12 C11 C16 C15 4(4) . .
C14 C15 C16 C11 -2(4) . .
O15 C17 C18 C19 177(2) . .
C22 C17 C18 C19 -1(3) . .
C17 C18 C19 C20 -7(4) . .
C18 C19 C20 C21 13(5) . .
C19 C20 C21 C22 -11(6) . .
C20 C21 C22 C23 -174(3) . .
C20 C21 C22 C17 3(4) . .
O15 C17 C22 C21 -175(2) . .
C18 C17 C22 C21 3(3) . .
O15 C17 C22 C23 3(3) . .
C18 C17 C22 C23 -179.8(17) . .
C21 C22 C23 N3 -174(3) . .
C17 C22 C23 N3 9(4) . .
N3 C24 C25 N4 -26(3) . .
N4 C26 C27 C28 -175(2) . .
N4 C26 C27 C32 6(3) . .
C32 C27 C28 C29 4(3) . .
C26 C27 C28 C29 -175.1(19) . .
C27 C28 C29 C30 -2(3) . .
C28 C29 C30 C31 2(3) . .
C29 C30 C31 C32 -4(3) . .
C30 C31 C32 O24 -174(2) . .
C30 C31 C32 C27 6(3) . .
C28 C27 C32 O24 175.0(19) . .
C26 C27 C32 O24 -6(3) . .
C28 C27 C32 C31 -5(3) . .
C26 C27 C32 C31 173.4(18) . .
C11 C10 N1 C9 176(2) . .
C11 C10 N1 Cu1 4(4) . .
C8 C9 N1 C10 -149(3) . .
C8 C9 N1 Cu1 24(3) . .
C6 C7 N2 C8 -175.0(19) . .
C6 C7 N2 Cu1 4(3) . .
C9 C8 N2 C7 -150(2) . .
C9 C8 N2 Cu1 31(3) . .
C22 C23 N3 C24 173(2) . .
C22 C23 N3 Cu2 -8(4) . .
C25 C24 N3 C23 -163(2) . .
C25 C24 N3 Cu2 17(3) . .
C27 C26 N4 C25 -176(2) . .
C27 C26 N4 Cu2 0(3) . .
C24 C25 N4 C26 -159(2) . .
C24 C25 N4 Cu2 24(3) . .
O23 O3 O3' Si1 -44.8(12) 5_557 .
W3 O3 O3' Si1 -179.7(13) . .
W4 O3 O3' Si1 -107(2) 5_557 .
W1 O3 O3' Si1 106(2) . .
Si1 O3 O3' W3 179.7(13) . .
O23 O3 O3' W3 134.9(15) 5_557 .
W4 O3 O3' W3 72.3(19) 5_557 .
W1 O3 O3' W3 -74.2(17) . .
Si1 O3 O3' W2 -100(2) . .
O23 O3 O3' W2 -144.7(19) 5_557 .
W3 O3 O3' W2 80.4(19) . .
W4 O3 O3' W2 152.7(14) 5_557 .
W1 O3 O3' W2 6(3) . .
Si1 O3 O3' W6 99(2) . .
O23 O3 O3' W6 54(2) 5_557 .
W3 O3 O3' W6 -80.7(18) . .
W4 O3 O3' W6 -8(3) 5_557 .
W1 O3 O3' W6 -154.9(14) . .
C18 C17 O15 Cu2 170.1(14) . .
C22 C17 O15 Cu2 -13(3) . .
C18 C17 O15 Cu3 -36(3) . .
C22 C17 O15 Cu3 141(2) . .
C31 C32 O24 Cu2 -179.1(14) . .
C27 C32 O24 Cu2 1(3) . .
C31 C32 O24 Cu3 37(3) . .
C27 C32 O24 Cu3 -143.4(17) . .
C2 C1 O25 Cu1 -179.8(18) . .
C6 C1 O25 Cu1 4(4) . .
C2 C1 O25 Cu3 35(4) . .
C6 C1 O25 Cu3 -141(2) . .
C11 C12 O27 Cu1 -10(3) . .
C13 C12 O27 Cu1 175.2(15) . .
C11 C12 O27 Cu3 132.3(19) . .
C13 C12 O27 Cu3 -42(3) . .
O3' O3 Si1 O3 -132(26) . 5_557
O23 O3 Si1 O3 -8(26) 5_557 5_557
W3 O3 Si1 O3 -132(26) . 5_557
W4 O3 Si1 O3 -7(26) 5_557 5_557
W1 O3 Si1 O3 108(26) . 5_557
O3' O3 Si1 O23 56.3(15) . .
O23 O3 Si1 O23 180.000(2) 5_557 .
W3 O3 Si1 O23 57(2) . .
W4 O3 Si1 O23 -178.8(13) 5_557 .
W1 O3 Si1 O23 -63.9(18) . .
O3' O3 Si1 O23 -123.7(15) . 5_557
W3 O3 Si1 O23 -123(2) . 5_557
W4 O3 Si1 O23 1.2(13) 5_557 5_557
W1 O3 Si1 O23 116.1(18) . 5_557
O23 O3 Si1 O3' 123.7(15) 5_557 .
W3 O3 Si1 O3' 0.4(15) . .
W4 O3 Si1 O3' 125(2) 5_557 .
W1 O3 Si1 O3' -120(2) . .
O3' O3 Si1 O3' 180.000(15) . 5_557
O23 O3 Si1 O3' -56.3(15) 5_557 5_557
W3 O3 Si1 O3' -179.6(15) . 5_557
W4 O3 Si1 O3' -55(2) 5_557 5_557
W1 O3 Si1 O3' 60(2) . 5_557
O3' O3 Si1 O2 -57.0(16) . 5_557
O23 O3 Si1 O2 66.7(14) 5_557 5_557
W3 O3 Si1 O2 -57(2) . 5_557
W4 O3 Si1 O2 67.9(18) 5_557 5_557
W1 O3 Si1 O2 -177.2(13) . 5_557
O3' O3 Si1 O2 123.0(16) . .
O23 O3 Si1 O2 -113.3(14) 5_557 .
W3 O3 Si1 O2 123(2) . .
W4 O3 Si1 O2 -112.1(18) 5_557 .
W1 O3 Si1 O2 2.8(13) . .
O3 O23 Si1 O3 180.000(2) 5_557 .
W4 O23 Si1 O3 -178.7(14) . .
W2 O23 Si1 O3 -50.6(17) . .
W5 O23 Si1 O3 61.3(16) . .
W4 O23 Si1 O3 1.3(14) . 5_557
W2 O23 Si1 O3 129.4(17) . 5_557
W5 O23 Si1 O3 -118.7(16) . 5_557
O3 O23 Si1 O23 90(100) 5_557 5_557
W4 O23 Si1 O23 92(100) . 5_557
W2 O23 Si1 O23 -140(100) . 5_557
W5 O23 Si1 O23 -28(100) . 5_557
O3 O23 Si1 O3' -127.5(15) 5_557 .
W4 O23 Si1 O3' -126.2(17) . .
W2 O23 Si1 O3' 1.9(13) . .
W5 O23 Si1 O3' 113.7(15) . .
O3 O23 Si1 O3' 52.5(15) 5_557 5_557
W4 O23 Si1 O3' 53.8(17) . 5_557
W2 O23 Si1 O3' -178.1(13) . 5_557
W5 O23 Si1 O3' -66.3(15) . 5_557
O3 O23 Si1 O2 -61.1(15) 5_557 5_557
W4 O23 Si1 O2 -59.8(16) . 5_557
W2 O23 Si1 O2 68.3(15) . 5_557
W5 O23 Si1 O2 -179.9(12) . 5_557
O3 O23 Si1 O2 118.9(15) 5_557 .
W4 O23 Si1 O2 120.2(16) . .
W2 O23 Si1 O2 -111.7(15) . .
W5 O23 Si1 O2 0.1(12) . .
W3 O3' Si1 O3 -0.4(16) . .
W2 O3' Si1 O3 124.3(19) . .
W6 O3' Si1 O3 -123.0(19) . .
O3 O3' Si1 O3 180.000(15) . 5_557
W3 O3' Si1 O3 179.6(16) . 5_557
W2 O3' Si1 O3 -55.7(19) . 5_557
W6 O3' Si1 O3 57.0(19) . 5_557
O3 O3' Si1 O23 -126.2(15) . .
W3 O3' Si1 O23 -126.6(19) . .
W2 O3' Si1 O23 -1.9(13) . .
W6 O3' Si1 O23 110.8(15) . .
O3 O3' Si1 O23 53.8(15) . 5_557
W3 O3' Si1 O23 53.4(19) . 5_557
W2 O3' Si1 O23 178.1(13) . 5_557
W6 O3' Si1 O23 -69.2(15) . 5_557
O3 O3' Si1 O3' -116(66) . 5_557
W3 O3' Si1 O3' -116(66) . 5_557
W2 O3' Si1 O3' 8(66) . 5_557
W6 O3' Si1 O3' 121(66) . 5_557
O3 O3' Si1 O2 124.5(16) . 5_557
W3 O3' Si1 O2 124.1(19) . 5_557
W2 O3' Si1 O2 -111.2(17) . 5_557
W6 O3' Si1 O2 1.5(13) . 5_557
O3 O3' Si1 O2 -55.5(16) . .
W3 O3' Si1 O2 -55.9(19) . .
W2 O3' Si1 O2 68.8(17) . .
W6 O3' Si1 O2 -178.5(13) . .
W1 O2 Si1 O3 -3.2(15) . .
W6 O2 Si1 O3 128.4(18) 5_557 .
W5 O2 Si1 O3 -120.0(17) . .
W1 O2 Si1 O3 176.8(15) . 5_557
W6 O2 Si1 O3 -51.6(18) 5_557 5_557
W5 O2 Si1 O3 60.0(17) . 5_557
W1 O2 Si1 O23 116.7(16) . .
W6 O2 Si1 O23 -111.8(16) 5_557 .
W5 O2 Si1 O23 -0.1(12) . .
W1 O2 Si1 O23 -63.3(16) . 5_557
W6 O2 Si1 O23 68.2(16) 5_557 5_557
W5 O2 Si1 O23 179.9(12) . 5_557
W1 O2 Si1 O3' 50.0(18) . .
W6 O2 Si1 O3' -178.4(14) 5_557 .
W5 O2 Si1 O3' -66.7(16) . .
W1 O2 Si1 O3' -130.0(18) . 5_557
W6 O2 Si1 O3' 1.6(14) 5_557 5_557
W5 O2 Si1 O3' 113.3(16) . 5_557
W1 O2 Si1 O2 -165(100) . 5_557
W6 O2 Si1 O2 -33(100) 5_557 5_557
W5 O2 Si1 O2 79(100) . 5_557
C12 O27 Cu1 N2 -48(9) . .
Cu3 O27 Cu1 N2 159(8) . .
C12 O27 Cu1 N1 10(2) . .
Cu3 O27 Cu1 N1 -142.7(8) . .
C12 O27 Cu1 O25 -178.7(19) . .
Cu3 O27 Cu1 O25 28.3(8) . .
C7 N2 Cu1 O27 -135(8) . .
C8 N2 Cu1 O27 44(9) . .
C7 N2 Cu1 N1 167(2) . .
C8 N2 Cu1 N1 -14.4(15) . .
C7 N2 Cu1 O25 -4(2) . .
C8 N2 Cu1 O25 174.9(15) . .
C10 N1 Cu1 O27 -7(2) . .
C9 N1 Cu1 O27 -179.5(17) . .
C10 N1 Cu1 N2 168(2) . .
C9 N1 Cu1 N2 -4.4(17) . .
C10 N1 Cu1 O25 -117(5) . .
C9 N1 Cu1 O25 70(6) . .
C1 O25 Cu1 O27 176(2) . .
Cu3 O25 Cu1 O27 -28.5(8) . .
C1 O25 Cu1 N2 0(2) . .
Cu3 O25 Cu1 N2 155.8(7) . .
C1 O25 Cu1 N1 -73(6) . .
Cu3 O25 Cu1 N1 82(5) . .
C23 N3 Cu2 O15 -2(2) . .
C24 N3 Cu2 O15 177.5(19) . .
C23 N3 Cu2 N4 177(2) . .
C24 N3 Cu2 N4 -3(2) . .
C23 N3 Cu2 O24 -118(9) . .
C24 N3 Cu2 O24 62(10) . .
C17 O15 Cu2 N3 11.2(18) . .
Cu3 O15 Cu2 N3 -150.0(8) . .
C17 O15 Cu2 N4 -158(15) . .
Cu3 O15 Cu2 N4 40(16) . .
C17 O15 Cu2 O24 -173.2(18) . .
Cu3 O15 Cu2 O24 25.6(8) . .
C26 N4 Cu2 N3 171(2) . .
C25 N4 Cu2 N3 -12.3(17) . .
C26 N4 Cu2 O15 -19(17) . .
C25 N4 Cu2 O15 157(15) . .
C26 N4 Cu2 O24 -4(2) . .
C25 N4 Cu2 O24 172.1(17) . .
C32 O24 Cu2 N3 -61(10) . .
Cu3 O24 Cu2 N3 90(9) . .
C32 O24 Cu2 O15 -177.0(19) . .
Cu3 O24 Cu2 O15 -26.0(8) . .
C32 O24 Cu2 N4 3.8(19) . .
Cu3 O24 Cu2 N4 154.8(8) . .
C32 O24 Cu3 O1W -3(2) . .
Cu2 O24 Cu3 O1W -154.2(10) . .
C32 O24 Cu3 O15 173(2) . .
Cu2 O24 Cu3 O15 22.4(8) . .
C32 O24 Cu3 O25 142.1(18) . .
Cu2 O24 Cu3 O25 -9(2) . .
C32 O24 Cu3 O27 97.5(19) . .
Cu2 O24 Cu3 O27 -53.1(9) . .
C32 O24 Cu3 O19 -88.1(19) . .
Cu2 O24 Cu3 O19 121.2(8) . .
C17 O15 Cu3 O1W -156(6) . .
Cu2 O15 Cu3 O1W 1(7) . .
C17 O15 Cu3 O24 -180(2) . .
Cu2 O15 Cu3 O24 -22.8(7) . .
C17 O15 Cu3 O25 -14(2) . .
Cu2 O15 Cu3 O25 142.6(9) . .
C17 O15 Cu3 O27 -83(2) . .
Cu2 O15 Cu3 O27 74.0(9) . .
C17 O15 Cu3 O19 82(2) . .
Cu2 O15 Cu3 O19 -121.2(8) . .
C1 O25 Cu3 O1W -85(3) . .
Cu1 O25 Cu3 O1W 122.5(10) . .
C1 O25 Cu3 O24 127(3) . .
Cu1 O25 Cu3 O24 -24.9(19) . .
C1 O25 Cu3 O15 100(3) . .
Cu1 O25 Cu3 O15 -52.4(9) . .
C1 O25 Cu3 O27 176(3) . .
Cu1 O25 Cu3 O27 23.8(7) . .
C1 O25 Cu3 O19 -4(3) . .
Cu1 O25 Cu3 O19 -156.0(7) . .
C12 O27 Cu3 O1W 92(2) . .
Cu1 O27 Cu3 O1W -117.4(10) . .
C12 O27 Cu3 O24 -17(2) . .
Cu1 O27 Cu3 O24 134.1(8) . .
C12 O27 Cu3 O15 -80(2) . .
Cu1 O27 Cu3 O15 70.6(8) . .
C12 O27 Cu3 O25 -175(2) . .
Cu1 O27 Cu3 O25 -24.4(7) . .
C12 O27 Cu3 O19 -175(2) . .
Cu1 O27 Cu3 O19 -24(3) . .
W1 O19 Cu3 O1W -32.8(18) . .
W1 O19 Cu3 O24 73.8(18) . .
W1 O19 Cu3 O15 140.1(18) . .
W1 O19 Cu3 O25 -128.4(18) . .
W1 O19 Cu3 O27 -129(3) . .
Cu3 O19 W1 O12 -132.5(17) . .
Cu3 O19 W1 O26 137.8(17) . .
Cu3 O19 W1 O18 -40.3(18) . .
Cu3 O19 W1 O21 50.0(19) . .
Cu3 O19 W1 O2 8(3) . .
Cu3 O19 W1 O3 -174.5(17) . .
W3 O12 W1 O19 -152.7(16) . .
W3 O12 W1 O26 -52.6(17) . .
W3 O12 W1 O18 107.3(17) . .
W3 O12 W1 O21 21(3) . .
W3 O12 W1 O2 40.4(18) . .
W3 O12 W1 O3 9.2(15) . .
W4 O26 W1 O19 155.1(17) 5_557 .
W4 O26 W1 O12 54.9(18) 5_557 .
W4 O26 W1 O18 -30(4) 5_557 .
W4 O26 W1 O21 -101.9(19) 5_557 .
W4 O26 W1 O2 -40.9(19) 5_557 .
W4 O26 W1 O3 -5.1(15) 5_557 .
W5 O18 W1 O19 163.2(14) . .
W5 O18 W1 O12 -96.1(15) . .
W5 O18 W1 O26 -11(3) . .
W5 O18 W1 O21 59.8(16) . .
W5 O18 W1 O2 0.1(13) . .
W5 O18 W1 O3 -34.1(16) . .
W6 O21 W1 O19 -152.7(18) 5_557 .
W6 O21 W1 O12 33(3) 5_557 .
W6 O21 W1 O26 107.7(19) 5_557 .
W6 O21 W1 O18 -53.1(19) 5_557 .
W6 O21 W1 O2 11.6(16) 5_557 .
W6 O21 W1 O3 44(2) 5_557 .
Si1 O2 W1 O19 -179.0(13) . .
W6 O2 W1 O19 41(3) 5_557 .
W5 O2 W1 O19 -54(2) . .
Si1 O2 W1 O12 -37.6(16) . .
W6 O2 W1 O12 -177.5(8) 5_557 .
W5 O2 W1 O12 87.8(8) . .
Si1 O2 W1 O26 50.6(15) . .
W6 O2 W1 O26 -89.4(10) 5_557 .
W5 O2 W1 O26 176.0(8) . .
Si1 O2 W1 O18 -125.5(17) . .
W6 O2 W1 O18 94.6(10) 5_557 .
W5 O2 W1 O18 -0.1(7) . .
Si1 O2 W1 O21 133.7(19) . .
W6 O2 W1 O21 -6.3(8) 5_557 .
W5 O2 W1 O21 -100.9(11) . .
Si1 O2 W1 O3 2.7(13) . .
W6 O2 W1 O3 -137.3(15) 5_557 .
W5 O2 W1 O3 128.1(14) . .
Si1 O3 W1 O19 178.7(11) . .
O3' O3 W1 O19 105(3) . .
O23 O3 W1 O19 -112(2) 5_557 .
W3 O3 W1 O19 43(2) . .
W4 O3 W1 O19 -51(2) 5_557 .
Si1 O3 W1 O12 130.7(19) . .
O3' O3 W1 O12 57(2) . .
O23 O3 W1 O12 -160(2) 5_557 .
W3 O3 W1 O12 -4.7(8) . .
W4 O3 W1 O12 -99.3(10) 5_557 .
Si1 O3 W1 O26 -127.3(19) . .
O3' O3 W1 O26 159(2) . .
O23 O3 W1 O26 -57.8(19) 5_557 .
W3 O3 W1 O26 97.3(11) . .
W4 O3 W1 O26 2.6(8) 5_557 .
Si1 O3 W1 O18 44.2(17) . .
O3' O3 W1 O18 -30(2) . .
O23 O3 W1 O18 113.7(19) 5_557 .
W3 O3 W1 O18 -91.2(9) . .
W4 O3 W1 O18 174.1(7) 5_557 .
Si1 O3 W1 O21 -44.3(18) . .
O3' O3 W1 O21 -118(2) . .
O23 O3 W1 O21 25(2) 5_557 .
W3 O3 W1 O21 -179.7(9) . .
W4 O3 W1 O21 85.6(9) 5_557 .
Si1 O3 W1 O2 -2.7(13) . .
O3' O3 W1 O2 -76(2) . .
O23 O3 W1 O2 66.9(19) 5_557 .
W3 O3 W1 O2 -138.1(16) . .
W4 O3 W1 O2 127.3(14) 5_557 .
W4 O11 W2 O1 150.7(16) . .
W4 O11 W2 O7 49.8(17) . .
W4 O11 W2 O8 -38(3) . .
W4 O11 W2 O6 -108.3(17) . .
W4 O11 W2 O23 -13.4(14) . .
W4 O11 W2 O3' -45.8(17) . .
W5 O7 W2 O1 -156.9(15) . .
W5 O7 W2 O11 -54.2(15) . .
W5 O7 W2 O8 101.1(15) . .
W5 O7 W2 O6 15(3) . .
W5 O7 W2 O23 3.3(13) . .
W5 O7 W2 O3' 39.8(16) . .
W3 O8 W2 O1 156.1(16) . .
W3 O8 W2 O11 -16(3) . .
W3 O8 W2 O7 -102.6(16) . .
W3 O8 W2 O6 54.1(16) . .
W3 O8 W2 O23 -36.6(16) . .
W3 O8 W2 O3' -6.4(14) . .
W6 O6 W2 O1 -153.6(18) . .
W6 O6 W2 O11 104.6(19) . .
W6 O6 W2 O7 34(3) . .
W6 O6 W2 O8 -52.1(19) . .
W6 O6 W2 O23 45.2(19) . .
W6 O6 W2 O3' 6.7(16) . .
Si1 O23 W2 O1 -177.7(16) . .
O3 O23 W2 O1 -106(3) 5_557 .
W4 O23 W2 O1 -37(2) . .
W5 O23 W2 O1 57(2) . .
Si1 O23 W2 O11 -134.1(16) . .
O3 O23 W2 O11 -62(2) 5_557 .
W4 O23 W2 O11 6.7(7) . .
W5 O23 W2 O11 101.0(9) . .
Si1 O23 W2 O7 123.2(15) . .
O3 O23 W2 O7 -165(2) 5_557 .
W4 O23 W2 O7 -96.0(9) . .
W5 O23 W2 O7 -1.7(7) . .
Si1 O23 W2 O8 36.0(14) . .
O3 O23 W2 O8 108(2) 5_557 .
W4 O23 W2 O8 176.8(7) . .
W5 O23 W2 O8 -88.9(7) . .
Si1 O23 W2 O6 -52.0(14) . .
O3 O23 W2 O6 20(2) 5_557 .
W4 O23 W2 O6 88.7(8) . .
W5 O23 W2 O6 -177.0(7) . .
Si1 O23 W2 O3' -1.7(12) . .
O3 O23 W2 O3' 70(2) 5_557 .
W4 O23 W2 O3' 139.0(14) . .
W5 O23 W2 O3' -126.7(13) . .
Si1 O3' W2 O1 177.8(15) . .
O3 O3' W2 O1 -114(3) . .
W3 O3' W2 O1 -44(3) . .
W6 O3' W2 O1 52(3) . .
Si1 O3' W2 O11 41.4(16) . .
O3 O3' W2 O11 110(2) . .
W3 O3' W2 O11 179.6(9) . .
W6 O3' W2 O11 -84.1(9) . .
Si1 O3' W2 O7 -47.2(16) . .
O3 O3' W2 O7 21(2) . .
W3 O3' W2 O7 90.9(9) . .
W6 O3' W2 O7 -172.7(8) . .
Si1 O3' W2 O8 -134.7(18) . .
O3 O3' W2 O8 -66(2) . .
W3 O3' W2 O8 3.5(7) . .
W6 O3' W2 O8 99.8(10) . .
Si1 O3' W2 O6 122.2(18) . .
O3 O3' W2 O6 -169(3) . .
W3 O3' W2 O6 -99.7(11) . .
W6 O3' W2 O6 -3.3(8) . .
Si1 O3' W2 O23 1.6(11) . .
O3 O3' W2 O23 70(2) . .
W3 O3' W2 O23 139.8(15) . .
W6 O3' W2 O23 -123.9(13) . .
W6 O9 W3 O16 155.7(18) . .
W6 O9 W3 O8 53.7(19) . .
W6 O9 W3 O10 -104.0(18) . .
W6 O9 W3 O12 -25(3) . .
W6 O9 W3 O3' -8.2(16) . .
W6 O9 W3 O3 -41(2) . .
W2 O8 W3 O16 -159.3(16) . .
W2 O8 W3 O9 -55.4(16) . .
W2 O8 W3 O10 31(3) . .
W2 O8 W3 O12 100.7(16) . .
W2 O8 W3 O3' 6.5(14) . .
W2 O8 W3 O3 38.1(16) . .
W4 O10 W3 O16 -156.4(16) 5_557 .
W4 O10 W3 O9 99.6(16) 5_557 .
W4 O10 W3 O8 13(3) 5_557 .
W4 O10 W3 O12 -56.4(15) 5_557 .
W4 O10 W3 O3' 35.4(16) 5_557 .
W4 O10 W3 O3 5.5(14) 5_557 .
W1 O12 W3 O16 152.1(17) . .
W1 O12 W3 O9 -28(3) . .
W1 O12 W3 O8 -106.6(17) . .
W1 O12 W3 O10 52.6(17) . .
W1 O12 W3 O3' -42.4(17) . .
W1 O12 W3 O3 -9.4(16) . .
Si1 O3' W3 O16 177(2) . .
O3 O3' W3 O16 177(3) . .
W2 O3' W3 O16 43(3) . .
W6 O3' W3 O16 -51(3) . .
Si1 O3' W3 O9 -128(2) . .
O3 O3' W3 O9 -127.8(16) . .
W2 O3' W3 O9 98.5(11) . .
W6 O3' W3 O9 4.3(8) . .
Si1 O3' W3 O8 131(2) . .
O3 O3' W3 O8 130.2(15) . .
W2 O3' W3 O8 -3.5(7) . .
W6 O3' W3 O8 -97.7(10) . .
Si1 O3' W3 O10 -40.3(18) . .
O3 O3' W3 O10 -40.7(13) . .
W2 O3' W3 O10 -174.3(8) . .
W6 O3' W3 O10 91.5(8) . .
Si1 O3' W3 O12 45.7(18) . .
O3 O3' W3 O12 45.4(13) . .
W2 O3' W3 O12 -88.2(9) . .
W6 O3' W3 O12 177.5(8) . .
Si1 O3' W3 O3 0.3(14) . .
W2 O3' W3 O3 -133.6(16) . .
W6 O3' W3 O3 132.1(16) . .
Si1 O3 W3 O16 -177.9(19) . .
O3' O3 W3 O16 -178(2) . .
O23 O3 W3 O16 106(3) 5_557 .
W4 O3 W3 O16 46(3) 5_557 .
W1 O3 W3 O16 -46(3) . .
Si1 O3 W3 O9 45.2(19) . .
O3' O3 W3 O9 45.5(14) . .
O23 O3 W3 O9 -31(2) 5_557 .
W4 O3 W3 O9 -90.6(9) 5_557 .
W1 O3 W3 O9 177.1(9) . .
Si1 O3 W3 O8 -44.1(18) . .
O3' O3 W3 O8 -43.7(13) . .
O23 O3 W3 O8 -120(2) 5_557 .
W4 O3 W3 O8 -179.8(8) 5_557 .
W1 O3 W3 O8 87.8(9) . .
Si1 O3 W3 O10 133(2) . .
O3' O3 W3 O10 133.4(15) . .
O23 O3 W3 O10 57(2) 5_557 .
W4 O3 W3 O10 -2.7(7) 5_557 .
W1 O3 W3 O10 -95.1(10) . .
Si1 O3 W3 O12 -127(2) . .
O3' O3 W3 O12 -127.1(15) . .
O23 O3 W3 O12 156(3) 5_557 .
W4 O3 W3 O12 96.8(10) 5_557 .
W1 O3 W3 O12 4.5(7) . .
Si1 O3 W3 O3' -0.4(14) . .
O23 O3 W3 O3' -76(2) 5_557 .
W4 O3 W3 O3' -136.1(16) 5_557 .
W1 O3 W3 O3' 131.6(17) . .
W2 O11 W4 O20 -147.8(17) . .
W2 O11 W4 O10 32(3) . 5_557
W2 O11 W4 O13 -50.2(17) . .
W2 O11 W4 O26 108.2(17) . 5_557
W2 O11 W4 O23 13.6(14) . .
W2 O11 W4 O3 44.1(17) . 5_557
W5 O13 W4 O20 158.1(16) . .
W5 O13 W4 O11 52.3(15) . .
W5 O13 W4 O10 -103.7(15) . 5_557
W5 O13 W4 O26 -32(3) . 5_557
W5 O13 W4 O23 -7.1(13) . .
W5 O13 W4 O3 -41.3(16) . 5_557
Si1 O23 W4 O20 -171(2) . .
O3 O23 W4 O20 -169(2) 5_557 .
W2 O23 W4 O20 52(3) . .
W5 O23 W4 O20 -41(3) . .
Si1 O23 W4 O11 131.2(17) . .
O3 O23 W4 O11 132.4(14) 5_557 .
W2 O23 W4 O11 -6.6(7) . .
W5 O23 W4 O11 -98.8(9) . .
Si1 O23 W4 O10 -41.2(15) . 5_557
O3 O23 W4 O10 -40.1(12) 5_557 5_557
W2 O23 W4 O10 -179.1(8) . 5_557
W5 O23 W4 O10 88.8(7) . 5_557
Si1 O23 W4 O13 -126.2(16) . .
O3 O23 W4 O13 -125.0(13) 5_557 .
W2 O23 W4 O13 96.0(9) . .
W5 O23 W4 O13 3.8(7) . .
Si1 O23 W4 O26 45.0(15) . 5_557
O3 O23 W4 O26 46.1(12) 5_557 5_557
W2 O23 W4 O26 -92.9(8) . 5_557
W5 O23 W4 O26 175.0(7) . 5_557
Si1 O23 W4 O3 -1.1(12) . 5_557
W2 O23 W4 O3 -139.0(14) . 5_557
W5 O23 W4 O3 128.9(13) . 5_557
W6 O14 W5 O22 155.4(17) 5_557 .
W6 O14 W5 O7 -24(4) 5_557 .
W6 O14 W5 O18 56.1(18) 5_557 .
W6 O14 W5 O13 -104.8(18) 5_557 .
W6 O14 W5 O2 -4.2(15) 5_557 .
W6 O14 W5 O23 -42.3(18) 5_557 .
W2 O7 W5 O22 157.1(15) . .
W2 O7 W5 O14 -24(3) . .
W2 O7 W5 O18 -103.1(15) . .
W2 O7 W5 O13 57.3(16) . .
W2 O7 W5 O2 -41.2(16) . .
W2 O7 W5 O23 -3.2(13) . .
W1 O18 W5 O22 -162.3(14) . .
W1 O18 W5 O14 -60.7(15) . .
W1 O18 W5 O7 98.4(15) . .
W1 O18 W5 O13 16(3) . .
W1 O18 W5 O2 -0.1(13) . .
W1 O18 W5 O23 33.9(15) . .
W4 O13 W5 O22 -154.8(15) . .
W4 O13 W5 O14 103.4(16) . .
W4 O13 W5 O7 -55.7(15) . .
W4 O13 W5 O18 27(3) . .
W4 O13 W5 O2 41.4(16) . .
W4 O13 W5 O23 6.9(12) . .
Si1 O2 W5 O22 179.5(13) . .
W1 O2 W5 O22 47(2) . .
W6 O2 W5 O22 -53(2) 5_557 .
Si1 O2 W5 O14 -125.4(16) . .
W1 O2 W5 O14 101.6(11) . .
W6 O2 W5 O14 2.3(8) 5_557 .
Si1 O2 W5 O7 47.6(14) . .
W1 O2 W5 O7 -85.3(9) . .
W6 O2 W5 O7 175.3(8) 5_557 .
Si1 O2 W5 O18 133.0(16) . .
W1 O2 W5 O18 0.1(7) . .
W6 O2 W5 O18 -99.3(10) 5_557 .
Si1 O2 W5 O13 -41.6(14) . .
W1 O2 W5 O13 -174.5(8) . .
W6 O2 W5 O13 86.1(9) 5_557 .
Si1 O2 W5 O23 0.1(10) . .
W1 O2 W5 O23 -132.8(13) . .
W6 O2 W5 O23 127.8(12) 5_557 .
Si1 O23 W5 O22 -179.5(13) . .
O3 O23 W5 O22 114(2) 5_557 .
W4 O23 W5 O22 45(2) . .
W2 O23 W5 O22 -51(2) . .
Si1 O23 W5 O14 46.4(14) . .
O3 O23 W5 O14 -19.9(18) 5_557 .
W4 O23 W5 O14 -89.6(8) . .
W2 O23 W5 O14 174.4(8) . .
Si1 O23 W5 O7 -126.3(15) . .
O3 O23 W5 O7 167(2) 5_557 .
W4 O23 W5 O7 97.7(9) . .
W2 O23 W5 O7 1.7(7) . .
Si1 O23 W5 O18 -41.1(13) . .
O3 O23 W5 O18 -107.4(18) 5_557 .
W4 O23 W5 O18 -177.1(7) . .
W2 O23 W5 O18 86.9(8) . .
Si1 O23 W5 O13 132.2(15) . .
O3 O23 W5 O13 65.8(18) 5_557 .
W4 O23 W5 O13 -3.9(7) . .
W2 O23 W5 O13 -99.8(9) . .
Si1 O23 W5 O2 -0.1(11) . .
O3 O23 W5 O2 -66.4(18) 5_557 .
W4 O23 W5 O2 -136.1(12) . .
W2 O23 W5 O2 127.9(12) . .
W2 O6 W6 O17 153.2(18) . .
W2 O6 W6 O21 -106.0(19) . 5_557
W2 O6 W6 O14 -26(4) . 5_557
W2 O6 W6 O9 51.1(19) . .
W2 O6 W6 O2 -45.9(19) . 5_557
W2 O6 W6 O3' -6.6(16) . .
W3 O9 W6 O17 -153.9(18) . .
W3 O9 W6 O6 -53.0(19) . .
W3 O9 W6 O21 26(4) . 5_557
W3 O9 W6 O14 105.3(19) . 5_557
W3 O9 W6 O2 41(2) . 5_557
W3 O9 W6 O3' 8.0(16) . .
Si1 O3' W6 O17 -179.1(16) . .
O3 O3' W6 O17 114(3) . .
W3 O3' W6 O17 44(3) . .
W2 O3' W6 O17 -53(3) . .
Si1 O3' W6 O6 -122.9(17) . .
O3 O3' W6 O6 170(2) . .
W3 O3' W6 O6 100.2(11) . .
W2 O3' W6 O6 3.5(8) . .
Si1 O3' W6 O21 -40.4(15) . 5_557
O3 O3' W6 O21 -108(2) . 5_557
W3 O3' W6 O21 -177.3(9) . 5_557
W2 O3' W6 O21 86.1(9) . 5_557
Si1 O3' W6 O14 49.8(15) . 5_557
O3 O3' W6 O14 -17(2) . 5_557
W3 O3' W6 O14 -87.1(9) . 5_557
W2 O3' W6 O14 176.3(9) . 5_557
Si1 O3' W6 O9 132.6(18) . .
O3 O3' W6 O9 65(2) . .
W3 O3' W6 O9 -4.3(8) . .
W2 O3' W6 O9 -100.9(11) . .
Si1 O3' W6 O2 -1.4(12) . 5_557
O3 O3' W6 O2 -69(2) . 5_557
W3 O3' W6 O2 -138.3(14) . 5_557
W2 O3' W6 O2 125.1(14) . 5_557
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 -0.006 0.398 0.000 1963.1 449.7
2 -0.156 0.813 0.500 1963.3 446.0
